of 22 /22
DEPARTMENT OF CIVIL ENGINEERING, IIT DELHI CEL 774 CONSTRUCTION PRACTISES CONSTRUCTION PRACTISES Mix design of Concrete: IS method B. Bhattacharjee CIVIL ENGINEERING DEPARTMENT IIT DELHI
• Author

others
• Category

## Documents

• view

2

0

Embed Size (px)

### Transcript of Improving Literacy Through School Libraries Grant, Masada

CEL 774 CONSTRUCTION PRACTISESCONSTRUCTION PRACTISES
Mix design of Concrete: IS method
B. Bhattacharjee
General Outline
B. Bhattacharjee
IS METHOD
Step 1: f m =f ck + 1.65σ
The standard deviations are: M10-M15: 3.5 MPa M20-M25: 4.0 MPa M30-M50: 5.0 MPa
DETERMINE FROM SITE DATA, 30 CUBES
B. Bhattacharjee
IS METHOD
B. Bhattacharjee
IS METHOD Step 2 :
B. Bhattacharjee
DEPARTMENT OF CIVIL ENGINEERING, IIT DELHI
Step 3: Estimate water content & sand contents for concrete grades up to M35up to M35/ above M35
IS METHOD
B. Bhattacharjee
m.s.a (mm) W kg/m3 p=Fagg Vol (%of Total)
10 208 40
20 186
40 165
Step 3: Estimate water content & sand contents for concrete grades up to M35/ above M35above M35
IS METHOD
B. Bhattacharjee
m.s.a (mm) W kg/m3 p=Fagg vol (%of Total)
10 200 28
2520 180
Step 3: Estimate water content & sand contents for concrete grades up to M35/ above M35
IS METHOD
B. Bhattacharjee
DEPARTMENT OF CIVIL ENGINEERING, IIT DELHI
The Tables are for: Crushed CA Fine aggregate Zone II w/c =0.6(up to M35) & 0.35 (>M35) Compaction factor =0.8
Step 3: Estimate water content & sand contents for concrete grades up to M35/ above M35 (Adjustments)
IS METHOD
B. Bhattacharjee
CF(±) 0.1 3%(±) 0 ±1%w/c (±) 0.05 0
Step 4: Calculate cement content, Aggregate contents,
w/cw/c*= Min (w/c*= Min (w/ccurvecurve, w/c, w/cdurabilitydurability) ) .. C=Max(W/ w/c*, Cdurability).
IS METHOD
1000 11
1000 1
)1( 1
m.s.a (mm) Air content (%)
IS METHOD (Example) M25 concrete
Cement 43 grade Moderate exposure Zone III sand Compaction factor 0.9 20 mm m.s.a rounded aggregate
B. Bhattacharjee
IS METHOD (Example)
31.6
TMS
25
4
SD
B. Bhattacharjee
w/c =0.43
B. Bhattacharjee
Exposure Min C Max w/c Min Grade
Mild 300 0.55
M 20
Moderate 300 M 25 Severe 320 M 30 Very severe 340 M 35 Extreme 360 M40
Step 2: w/c*=0.43,
Step 3: Estimate water content & sand contents for concrete grades up to M35up to M35/ above M35
IS METHOD
B. Bhattacharjee
m.s.a (mm) W kg/m3 p=Fagg(%of Total)
10 208 40
Δ p (%)=-1.5+(0.43-0.6)×0.01/0.05-7=-11.9
IS METHOD
B. Bhattacharjee
CF(±) 0.1 3%(±) 0 ±1%w/c (±) 0.05 0
Step 4: w/cw/c*= Min (0.43, 0.50)=0.43 .*= Min (0.43, 0.50)=0.43 . W=186-9.2≈177kg/m3
C=Max(177/ 0.43, 300). =411.6≈412 kg/m3
IS METHOD
1000 1
7.2231.0 1
15.3 412177)02.01( ×
1000 1
6.2)231.01( 1
15.3 41217798.0 ×
p= 35p= 35--11.9=23.111.9=23.1 FFaggagg=419.25 kg/m=419.25 kg/m33
CCaggagg= 1344.0kg/m= 1344.0kg/m33
W=186-9.2≈177kg/m3
IS METHOD
B. Bhattacharjee
FFaggagg=419.25 kg/m=419.25 kg/m33
CCaggagg= 1344.0kg/m= 1344.0kg/m33
Total= 2352 kg/mTotal= 2352 kg/m33
Actual water to be added =177-water (present – absorption) in aggregate in kg/m3
Actual quantity of aggregate in the mix shall be Aggregate content + extra due to (moisture content- absorption)
IS METHOD
B. Bhattacharjee